Summary of the experimental results of the reviewed publications involving origin and size of CNCs, and mechanical properties of electrospun nanocomposite fibers/mats.
Cellulose, one of the world’s most abundant, natural and renewable biopolymer resources, is widely present in various forms of biomasses, such as trees, plants, tunicate and bacteria. Cellulose molecule consists of β-1, 4-D-linked glucose chains with molecular formula of (C6H10O5)n (n ranging from 10,000 to 15,000) through an acetal oxygen covalently bonding C1 of one glucose ring and C4 of the adjoining ring (O Sullivan, 1997; Samir et al., 2005). In plant cell walls, approximately 36 individual cellulose molecule chains connect with each other through hydrogen bonding to form larger units known as elementary ﬁbrils, which are packed into larger microfibrils with 5-50 nm in diameter and several micrometers in length. These microfibrils have disordered (amorphous) regions and highly ordered (crystalline) regions. In the crystalline regions, cellulose chains are closely packed together by a strong and highly intricate intra- and intermolecular hydrogen-bond network (Figure 1), while the amorphous domains are regularly distributed along the microﬁbrils. When lignocellulosic biomass are subjected to pure mechanical shearing, and a combination of chemical, mechanical and/or enzymatic treatment (Beck-Candanedo et al., 2005; Bondeson et al., 2006; Filson et al., 2009), the amorphous regions of cellulose microfibrils are selectively hydrolyzed under certain conditions because they are more susceptible to be attacked in contrast to crystalline domains. Consequently, these microﬁbrils break down into shorter crystalline parts with high crystalline degree, which are generally referred to as cellulose nanocrystals (CNCs) (Habibi et al., 2010). CNCs are also named as microcrystals, whiskers, nanoparticles, microcrystallites, nanofibers, or nanofibrils in the liturautes, all of which are called “cellulose nanocrystals” in this review.
During the past decade, CNCs have attracted considerable attention attributed to their unique features. First, CNCs have nanoscale dimensions and excellent mechanical properties. The theoretical value of Young’s modulus along the chain axis for perfect native CNCs is estimated to be 167.5 GPa, which is even theoretically stronger than steel and similar to Kevlar (Tashiro & Kobayashi, 1991), while elastic modulus of native CNCs from cotton and tunicate reach up to 105 and 143 GPa, respectively (Rusli & Eichhorn, 2008; Sturcova et al., 2005). Due to an abundance of hydroxyl groups existed on surface of CNCs, reactive CNCs can be modified with various chemical groups to accomplish expected surface modification, such as esteriﬁcation, etheriﬁcation, oxidation, silylation, or polymer grafting, which could successfully functionalize the CNCs and facilitate the incorporation and dispersion of CNCs into different polymer matrices (Habibi et al., 2010). Therefore, CNCs are considered as one of the ideal nano-reinforcements for polymer matrices (including water-soluble and water-insoluble polymer systems) and have already been incorporated into many polymer matrices to produce reinforced composites (Cao et al., 2011; Kvien et al., 2005). In addition, high aspect ratio, low density, low energy consumption, inherent renewability, biodegradability and biocompatibility are also the advantages of environmentally-friendly CNCs (Siro & Plackett, 2010). Because of the growing interest in the bioconversion of renewable lignocellulosic biomass and unsurpassed quintessential physical and chemical properties of CNCs mentioned above, substantial academic and industrial interests have been directed toward the potential applications of CNCs in polymer-based nanocomposites for various fields, such as high performance materials, electronics, catalysis, biomedical, and energy (Duran et al., 2011; Mangalam et al., 2009).
Many different approaches to fabricate polymer/CNCs nanocomposites have been reported (Eichhorn, 2011; Habibi et al., 2010; Moon et al., 2011), and most researches focused on conventional film materials (Peng et al., 2011). Recently, several non-conventional routes of producing polymer/CNCs nanocomposites have been reported, and some of the most exciting developments have been CNC-filled nanocomposite hydrogels (Capadona et al., 2009; Capadona et al., 2008; Shanmuganathan et al., 2010; Zhou et al., 2011b; Zhou et al., 2011c) and electrospun nanofibers (Lu et al., 2009; Martinez-Sanz et al., 2011; Medeiros et al., 2008; Park et al., 2007; Peresin et al., 2010b; Rojas et al., 2009; Xiang et al., 2009; Zhou et al., 2011a; Zoppe et al., 2009). These approaches could help expand novel applications of natural biomass nanocrystals in tissue engineering scaffolds, drug delivery, electronic components and devices.
This review is aim at presenting a summary on recent development of cellulose nanocrystals applied in advanced polymer-based nanocomposites using the novel fabrication strategies for targeting nanocomposite hydrogels and electrospun fibers. Specific attentions will be given to highlight opportunities of above-mentioned nanocomposites for future research.
2. Nanocomposite polymer hydrogels
The nanocomposite polymer hydrogels (NPHs), referred to cross-linked polymer networks swollen with water in the presence of nanoparticles or nanostructures, are new generation materials that can be used in a wide variety of applications including stimuli-responsive sensors and actuators, microfluidics, catalysis, separation devices, pharmaceutical, and biomedical devices (Schexnailder & Schmidt, 2009). The most potential use of NPHs is for novel biomaterials in tissue engineering, drug delivery, and hyperthermia treatment because they, in comparison with conventional hydrogels, can provide improved properties such as increased mechanical strength and ability for remote controlling (Samantha A. Meenach, 2009). Because of the excellent dispersion of CNCs in water (Liang et al., 2007), the fabrication, molding, and application of hydrogels containing CNCs without modification have many advantages compared with other nanofillers such as polymer and metal nanoparticles (Saravanan et al., 2007; Wu et al., 2009). Moreover, CNCs possessed the long-term biocompatibility and controlled biodegradability, which is beneficial to further develop applications of NPHs used as biomaterials.
Nakayama et al (2004) for the first time reported cellulose-polymer nanocomposite hydrogels composed of bacterial cellulose (BC) and gelatin. Bacterial cellulose is biosynthesized by microorganisms, and displays unique properties, including high mechanical strength, high water absorption capacity, high crystallinity, and an ultra-fine and highly pure fiber (10-100 nm) network structure (Vandamme et al., 1998). By immersing BC gel in aqueous gelatin solution followed by cross-linking with
By employing rod-shaped CNCs (about 10 nm in diameter and 120 nm in length) as the reinforcement nanofiller and in situ free-radical polymerizing/cross-linking acrylamide, we have successfully fabricated PAM-CNC nanocomposite hydrogels (Zhou et al., 2011b). During the gelation reaction of nanocomposite hydrogels, CNCs can accelerate the formation of hydrogels and then increased the effective crosslink density of hydrogels through the grafting copolymerization of monomer acrylamide on the surface of CNCs. Compared to the pure PAM hydrogels, the obtained nanocomposite hydrogels at a low loading level (6.7 wt%) of CNCs exhibited a dramatic enhancement in the shear storage modulus (4.6-fold) and the compression strength (2.5-fold). Hence, CNCs are not only a reinforcing agent for hydrogels, but also act as a multifunctional cross-linker for gelation. A possible mechanism for forming NPHs was proposed, as shown in Figure 2. Moreover, CNCs with smaller dimension and aspect ratios could help promote the sol-gel transition and facilitate the formation of nework of PAM-CNC nanocomposite hydrogels (Zhou et al., 2011c).
Spagnol et al (2012a) synthesized superabsorbent nanocomposite hydrogels based on poly(acrylamide-co-acrylate) (PAM-AA) and CNCs by free-radical aqueous copolymerization, and focused on the investigation of pH-responsiveness and cation-sensitivity character of NPHs. Swelling capacity and swelling-deswelling behavior of PAM-AA/CNC nanocompoiste hydrogel exhibited high pH-sensitivity and reversible pH-responsiveness properties. Furthermore, the swelling measurement in different salt solutions showed that the swelling capacity of NPHs in MgCl2 and CaCl2 solutions are much lower than that in NaCl and KCl solutions and distillated water. The swelling–deswelling process of NPHs was alternatively carried out between sodium and calcium solutions, suggesting a swelling-deswelling pulsatile behavior. It was reported that the pH and salt responsive behavior also occurred in superabsorbent nancomposite hydrogels based on CNCs and chitosan-graft-poly(acrylic acid) copolymer (Spagnol et al., 2012b).
PAM and its derivative hydrogels have been of great interest for developing applications in tissue engineering because of their non-toxic and biologically inertness, capability for preserving their shape and mechanical strength, and convenient adjustability of mechanical, chemical and biophysical properties (Zhou & Wu, 2011; Zhou et al., 2011d). Recently, we investigated the proliferations of dental follicle stem cells on PAM hydrogel and PAM/CNC nanocomposite hydrogel by alamarBlue® assay. As shown in Figure 3, the cell proliferations on PAM-CNC nanocomposite hydrogels were significantly higher than on the PAM hydrogels at days of 7 and 10, indicating that CNCs could help accelerate the proliferation of stem cells likely because the embedded nanocrystals formed an extracellular matrix-like microstructure in the hydrogel to promote cell-matrix interactions by providing more binding sites for cell adhesion and proliferation. This suggests that CNCs reinforced nanocomposite hydrogel systems showed improved cell biocompatibility and are suitable substrates used as cell carriers and traditional bone-defect repair and bone tissue engineering.
Aouada et al (2011) reported a simple, fast, and low cost strategy for the synthesis of nanocomposites by directly immerseing dry polyacrylamide-methylcellulose (PAM-MC) hydrogels into CNC aqueous suspensions. The CNCs were effectively anchored into the hydrogel network to provoke the increase in rigidity of the hydrogel networks and the decrease in pore sizes and the formation of three dimensional well-oriented pores. The incorporation of CNCs improved the crystallinity, and the mechanical and structural network properties of nanocomposite hydrogels without negatively impacting their thermal and hydrophilic properties. The value of the maximum compressive stress increased to 4.4 kPa for nanocomposite hydrogels from 2.1 kPa for pure PAM-MC hydrogels. Because of their biodegradability and biocompatibility, these reinforced nanocomposite hydrogels are promising materials for different technological applications, especially in agricultural applications, such as a carrier vehicle for agrochemical controlled release, such as pesticides (Aouada et al., 2010) and nutrients (Bortolin et al., 2012).
3. Electrospun nanocomposite fibers
Electrospinning is a highly versatile technique to generate continuous 1D polymeric fibers with diameters ranging from several micrometers down to 100 nanometers or less through a high voltage charged polymer solutions or melts (Reneker & Yarin, 2008). Electrospun nanofibrous materials possess a variety of interesting characteristics such as small dimension, large specific surface area, wide-range porosity, unique physicochemical property, and excellent flexibility for chemical/physical surface functionalization. Hence, electrospun nanofibrous materials not only are being used in research laboratories but also are increasingly applied in industry (Greiner & Wendorff, 2007). Their application includes, but is not limited to, optoelectronics, sensors, catalysis, filtration, energy-related materials and medicine. Electrospun polymeric nanofibers, however, are not sufficiently strong for many applications because of low molecular chain orientation along the fiber long-axis resulting from low stretching forces in the process of fiber formation (Ayutsede et al., 2006). During the past several years, a large number of studies have been conducted to improve mechanical properties of electrospun polymeric nanofibers. Incorporating nanoparticles into polymer matrices is one technique that has been developed and used as one of the most effective methods for reinforcing electrospun nanofibers (Hou et al., 2005; Lu et al., 2009). As one of the strongest and stiffest natural biopolymers, CNCs have been successfully used as highly effective reinforcing nanofillers for improving mechanical properties of various electrospun polymer matrices, as summarized in Table 1. Moreover, research effort has been focused on increased dispersion of CNCs in the matrix, improved alignment of CNCs along the fiber length, tailored CNC-matrix interfacial properties (Moon et al., 2011). According to the origination of polymer (i.e. synthetic and natural polymer), this section will concentrate on the processing of electrospun nanocomposite fibers and the effect of CNCs on their mechanical properties.
3.1. CNCs reinforced synthetic polymer
Due to the excellent dispersion property of CNCs in water, the first report of electrospun nanocomposite fibers was to electrospin water-soluble PEO and CNCs from BC. Highly crystalline rod-like CNCs with a high aspect ratio and specific area (420 ± 190 nm in length and 11 ± 4 nm in width) were incorporated into the electrospun PEO fibers with a diameter of less than 1 μm. Well-embedded CNCs were aligned and partially clustered inside the fibers. Compared with the electrospun PEO fibrous mats, the tensile modulus, tensile strength and elongation of electrospun nanocomposite fibrous mats containing 0.4 wt% of CNCs were increased by 193.9%, 72.3% and 233.3%, respectively, indicating that the existence of CNCs effectively improved the mechanical properties of the electrospun mats.
The dispersion of CNCs in electrospun fibers could be improved by tailoring the geometrical dimensions (length,
|Matrix||CNC origin and size||φCNC|
|PEO||Bacteria, 11 ± 4 nm in ||0–0.4||+193.9||+ 72.3||+233.3||(Park et al., 2007)|
+ 5658.6 a
- 99.9 a
|(Lu & Hsieh, 2009)|
|PEO||MCC, 10 ± 3 nm in ||0–20||+ 152.0|
+ 240.8 b
- 37.5 b
|(Zhou et al., 2011a)|
|PEO||Cotton, 5–10 nm in ||0–20||+ 190.5||+ 377.5||- 33.5||(Zhou et al., 2012b)|
|PEO||Tunicate, ~ 20 nm in ||0–15||+ 98.8c||―||―||(Changsarn et al., 2011)|
|PVA||Ramie, 3–10 nm in ||0–15||+ 270.9c||―||―||(Peresin et al., 2010b)|
|PCL||Ramie, 3–10 nm in ||0–7.5||+ 64.3|
|(Zoppe et al., 2009)|
|PS||Paper, 10–20 nm in ||0–9||+ ~60c||―||―||(Rojas et al., 2009)|
|PMMA||Bacteria, 15–20 nm in ||0–20||―||―||―||(Olsson et al., 2010)|
|PMMA||Wood, ~17 nm in ||0–41||+ 17d||―||―||(Dong et al., 2012)|
|PLA||MCC, 92 ± 3 nm in ||0–10||+ 37.0||+ 30.2||-1.4||(Xiang et al., 2009)|
|EVOH||Bacteria, lower than 30 nm in ||0–8||―||―||―||(Martinez-Sanz et al., 2011)|
|Silk||Bark, 25–40 nm in ||0–4||+ 300.3||+ 208.0||- 55.6||(Huang et al., 2011)|
For the hydrophobic polymer systems, CNCs should firstly be well-dispersed in organic solvent (such as DMF, N,N’-dimethylformamide; THF, tetrahydrofuran) before electrospinning because solution-based processing of nanocomposite nanofibers require good dispersability of both CNCs and polymer in one common solvent. Direct ultrasonication of freeze-dried CNCs is a facile method to prepare electrospinning solution (Xiang et al., 2009), and the redispersion of CNCs could be improved by conducting surface modification on CNCs (Zoppe et al., 2009) and adding additves. Rojas et al (2009) obtained fibers with smooth surface using solely THF as a solvent to electrospin PS containing surfactant-dispersed CNCs. The addition of non-ionic surfactant to the PS-CNC suspensions improved their stability, minimized (or prevented) the presence of beads in the resulting fibers, and promoted the nano-reinforcement of CNCs on PS fibers. However, the directly re-dispersed CNCs cannot form stable suspension at high loading leverls because the hydrophilic nature of cellulose and the strong hydrogen bonding interactions between CNCs. Olsson et al (2010) reported a two-step solvent exchange method to replace the water of CNC suspension by acetone, followed by further replacement through DMF/THF solvent in the same manner. A high degree of dispersion of CNCs was obtained for a variety of CNC contents and the aggregation of CNCs up to 7 wt% was greatly suppressed because CNCs were aligned and rapidly sealed inside PMMA matrix during the continuous formation of electrospun fibers. Moreover, the direct solvent exchange from water to organic solvent conducted by vacuum rotary evaporation was also used to disperse CNCs (Dong et al., 2012; Zoppe et al., 2009).
The alignment of CNCs along the fiber is also an important factor to determine the axial strength of electrospun nanocomposite fibers reinforced with CNCs. Considering CNCs can be aligned under the high electrostatic fields (Habibi et al., 2008), the electrospinning process could facilitate alignment of CNCs along the fiber long-axis. Usually, the alignment of CNCs was observed by scanning electron microscope (SEM) (Dong et al., 2012; Olsson et al., 2010) and TEM (Changsarn et al., 2011; Lu & Hsieh, 2009; Park et al., 2007; Zhou et al., 2011a). Figure 4 presents typical TEM pictures of CNC aligned parallel inside/along the longitudal axis of nanocomposite fibers. Interestingly, Figure 4b shows that CNCs dispensed in electrospun fibers had radial anisotropy or a skin-core morphology, in which CNCs in the core are oriented more randomly, while ones in the skin have a higher degree of orientation. Dong et al (2012) investigated the orientation of CNCs embedded in electrospun PMMA/CNC fiber by solvent-etching PMMA from nanocomposite fibers with drops of THF, and discovered highly aligned CNCs along the fiber axis, as shown in Figure 5. Besides the high electrostatic fields, the high alignment of CNCs along the polymer fiber could also be attributed to the shear forces in the liquid jet and the orientation of polymer chains during electrospinning process, and the nanoscale confinement effect (Chen et al., 2009).
It is well known that the improved interface between nanofillers with polymer matrix is beneficial to the mechanical properties of polymer-based nanocomposites (Zhang et al., 2010; Zhou et al., 2012a; Zhou et al., 2008b; Zhou et al., 2008c). For hydrophilic polymers, the hydrogen bonding between CNCs and polymer matrix play a very important role in determining polymer-CNC interaction. Peresin et al (Peresin et al., 2010b) reported CNC-reinforced nanocomposite fibers produced via electrospinning of poly(vinyl alcohol) (PVA) with two different concentrations of acetyl groups. The hydrogen bonding between PVA and CNCs was confirmed by observing the band between 3550 and 3200 cm-1 in Fourier transform infrared spectra (FTIR). The higher the hydrolysis degree of PVA (i. e. more –OH group in PVA chain), the stronger the PVA-CNC interaction, which was also observed by FTIR spectra. To confirm the effect of the hydrogen bonding, DMA in tensile mode was used for mechanical analysis. The storage modulus of nanocomposite fibrous mats showed a steady increase with increased CNC content from 0 to 15% loading. The storage modulus was 15.45 MPa for pure PVA mats and rose to 57.30 MPa at 15 wt% CNC loading. It was concluded that the observed strength enhancement in CNC-loaded PVA mats mainly is related to the reinforcing effect of the dispersed CNCs through the percolation network held by hydrogen bonds.
In addition to strong hydrogen bonding, covalent bonding also provides a means for enhancing polymer-nanofiller interface to achieve optimal composite properties (Zhou et al., 2008a). To produce greater reinforcing effect from CNCs in electrospun nanocomposite fibers, Lu & Hsieh (2009) fabricated electrospun PAA-CNC nanocomposite fibers. The interfacial interactions between CNCs and PAA could be further improved by heat-induced esterification between the CNC surface hydroxyls and PAA carboxyl groups, which produce covalent crosslinks at the PAA-CNC interfaces, render the nanocomposite fibrous mats insoluble in water, and make mats to be more thermally stable and far more superior tensile properties. The Young’s modulus and tensile strength of mats were significantly improved with increased CNC loadings in the nanocomposite fibers by up to 35-fold and 16-fold, respectively, with 20 wt% CNC loading, as shown in Figure 6. It is more impressive that the crosslinked nanocomposite fibrous mats with 20 wt% CNC exhibited 77-fold increase in modulus and 58-fold increase in strength, respectively. Moreover, the synergies of polymer crosslinking network and CNC‘s reinforcement could also improve the mechanical properties of nanocomposite fibrous mats. Recently, we reported UV-initiated crosslinking of PEO nanofibers in the presence of CNCs, which was performed with pentaerythritol triacrylate as both photo-initiator and crosslinker (Zhou et al., 2012b). With increased CNC content up to 10 wt%, the maximum tensile stress and Young's modulus of the crosslinked PEO/CNC composite fibrous mats increased by 377.5 and 190.5% than those of uncrosslinked PEO mats, and 76.5 and 127.4% than those of crosslinked PEO mats, respectively.
Due to the fact that the electrospun mats are non-woven fabrics, their mechanical properties are influenced by several factors including composition, morphology and structure of individual fiber, the interaction between fibers, orientation of fibers, and porosity of mats. An nano-indentation study was performed on single sub-micron PMMA/CNC fibers in the transverse direction to explore the reinforcement of CNCs on single nanocomposite fibers, which showed a modest increase in the mechanical properties with increasing CNC content, about 17% improvement in nano-DMA storage modulus with the loading of 17 wt% CNCs (Dong et al., 2012). In addition to the reinforceing effect of CNCs on fibers, it was also found that the addition of CNCs could reduce electrospun fiber diameters and improved fiber uniformity attributed to the enhanced electric conductivity of electrospinning solutions in the presence of CNCs. This tends to increase the mechanical properties of mats because smaller fiber diameters yield higher overall relative bonded areas between fibers by increasing its surface area, bonding density, and distribution of bonds (Olsson et al., 2010; Peresin et al., 2010b; Zhou et al., 2011a). Moreover, the orientation of nanocomposite fibers within mats also influence greatly on the mechanical properties of mats (Wang et al., 2011). Alignment of electrospun nanocomposite fibers reinforced with CNCs has been achieved by many techniques, including by running the fibers over a hollow spool with high rotation (Olsson et al., 2010), an aluminium frame with openings (Changsarn et al., 2011), a rotating mandrel covered with aluminium foil (Dong et al., 2012). Figure 5a shows the morphology of one-dimensional aligned fibers of PMMA/CNC. Furthermore, the more sufficient contact and stronger bonding between fibers could also lead to the improvement in mechanical properties of fibrous mats. It was found that humidity treatments on the PVA/CNC nanocomposite fibrous mats induced significant enhancement of strength as a result of the increased contact area and enhanced adhesion between the fibers (Peresin et al., 2010a). The heterogeneous fibrous mats composed of rigid–flexible bimodal PEO/CNC nanocomposite fibers was demonstrated to be higher in mechanical properties than their homogeneous counterparts (Zhou et al., 2011a). The reinforced mechanism was illustrated by morphology observation of the tensile process, as shown in Figure 7. With increased strain, the tensile stress of unaligned electrospun fibrous mats increased sharply at the beginning, and then increased slowly over a relatively long period of strain followed by the final rupture (Gomez-Tejedor et al., 2011). At the beginning of tensile process, the mats were stretched in a macroscopic view and most fibers in mats hardly moved attributed to the cohesion between fibers, which could determine Young’s modulus of mats. When most fibers in mats reached the tightened form, yield of mats appeared, at which the interaction points among fibers were broken. With further increase of tensile strain, the fibers in mats were drawn out to highly align along the tensile direction. However, the rupture of individual fibers one by one did not influence the tensile properties of the whole mats, resulting in a large elongation at break for electrospun mats. At the maximum tensile stress level, most fibers were necked and broken, leading to the final rupture of mats.
3.2. CNCs reinforced natural polymer
With increasing environmental consciousness about petroleum-based polymer materials, development of fully biodegradable, eco-friendly, and sustainable, bio-based nanocomposites have attracted more and more attention both in the academic and industrial fields (Kim & Netravali, 2010; Oksman et al., 2006). The so-called “green” composites are derived from natural resources including plant or animal origin (Khalil et al., 2012). Some researchers have successfully used CNCs as highly effective reinforcing nanofillers to fabricate electrospun bio-nanocomposite fibers from various biopolymers such as PLA (Li, 2010; Ramirez, 2010; Xiang et al., 2009), cellulose and its derivative (Herrera Vargas, 2010; Magalhaes et al., 2009), silk (Huang et al., 2011), and lignin (Ago et al., 2012).
PLA is such typical bio-based aliphatic polyester produced by polymerization of lactic acid, which is originated from renewable natural resources such as corn, starch, and molasses. The electrospun PLA/CNC nanocomposite fibers were widely reported because PLA possessed excellent physical properties of transparency, high elastic modulus, and high melting temperature. Xiang el al (2009) incorporated CNCs into electrospun PLA fibers, and found that Young’s modulus and strength of obtained nanocomposite mats with 1 wt% loading of CNCs were improved by approximately 37 and 30 %, respectively. Besides the reinforcement of CNCs on PLA fibers, Ramírez (2010) also investigated the cytocompatibility of the PLA/CNC nanocomposite fibrous mats used as scaffold. After one week of cell culture, confocal microscopy indicated that the cells grown on the PLA/CNC nanocomposite mats were confluent and very well aligned along the fibers while cells cultured on pure PLA mats were not as confluent as in the developed nanocomposite mats. This demonstrates the feasibility of the PLA/CNC nanocomposite fibrous mats as a potential scaffold for bone tissue engineering.
Magalhães et al (2009) reported a electrospun fully-cellulosic core-in-shell nanocomposite fibers consisting of regenerated cellulose (type II and amorphous) in the shell and CNCs in the core, which were fabricated by the co-electrospinning technique. Wood-based cellulose was dissolved in
4. Conclusion and perspectives for the future
In the review, recent development on applications of cellulose nanocrystals in nanocomposites fabricated by two novel strategies, i.e., gelation and electrospinning is presented. It is shown that CNCs have a distinct advantage for improving mechanical properties of both nanocomposite hydrogels and electrospun nanocomposite fibers/mats. The obviously reinforced effect of CNCs could help facilitate the potential applications of CNC-filled nanocompsite as advanced function materials.
CNCs reinforced hydrogels have been reported widely, and their properties, mainly mechanical properties, have been investigated. With the increased requirement for the multifunctional properties, nanocomposite hydrogels from CNCs and other stimuli-responsive polymer would be further developed. Various nanocomposite hydrogels reinforced with CNCs can be designed to become fast temperature, pH, and salt sensitive for controllable drug delivery system. Futhermore, using CNCs to reinforce natural polymer-based hydrogels could endow many favorable properties such as hydrophilicity, biodegradability, biocompatibility, low cost, and non-toxicity, resulting in applications of nanocomposite hydrogels in tissue engineering.
For the electrospun nanocomposite fibers containing CNCs, most studies focus on their fabrication, morphology, mechanical and thermal properties. There are still several major challenges for the further development of CNC-reinforced nanocomposites fibers. These include surface modification and homogeneous dispersion of CNCs, interface and alignment characterization of CNCs within individual electrospun nanocomposite fiber, analytical model for mechanics of single nanocomposite fiber, and assembly and effect of nanocomposite fibers within mats. More importantly, it is very worthwhile to exploit the functional characteristics and properties of CNC-filled nanocompsite fibers/mats to create new and specific applications such as energy-related materials, sensor, barrier films, and tissue engineering scaffolds.Acknowledgement
The authors would like to acknowledge the financial support from Louisiana Board of Regents Industrial Tie Subprogram (LEQSF(2010-13)-RD-B-01) and the USDA Rural Development Biomass Initiative Program (68-3A75-6-508). Special thanks go to Mrs. Maryam Rezai Rad and Dr. Shaomian Yao for their assistance in the cell culture of PAM/CNC nanocomposite hydrogels.
Ago M. Okajima K. Jakes J. E. Park S. Rojas O. J. 2012Lignin-Based Electrospun Nanofibers Reinforced with Cellulose Nanocrystals. 13 3 918 926
Aouada F. A. de Moura M. R. Orts W. J. Mattoso L. H. C. 2010Polyacrylamide and methylcellulose hydrogel as delivery vehicle for the controlled release of paraquat pesticide. 45 18 4977 4985
Aouada F. A. de Moura M. R. Orts W. J. Mattoso L. H. C. 2011Preparation and Characterization of Novel Micro- and Nanocomposite Hydrogels Containing Cellulosic Fibrils. 59 17 9433 9442
Ayutsede J. Gandhi M. Sukigara S. Ye H. H. Hsu C. M. Gogotsi Y. Ko F. 2006Carbon nanotube reinforced Bombyx mori silk nanofibers by the electrospinning process. 7 1 208 214
Beck-Candanedo S. Roman M. Gray D. G. 2005Effect of reaction conditions on the properties and behavior of wood cellulose nanocrystal suspensions. 6 2 1048 1054
Bochek A. M. 2008Prospects for use of polysaccharides of different origin and environmental problems in processing them. 40 3 192 197
Bondeson D. Mathew A. Oksman K. 2006Optimization of the isolation of nanocrystals from microcrystalline cellulose by acid hydrolysis. 13 2 171 180
Bortolin A. Aouada F. A. de Moura M. R. Ribeiro C. Longo E. Mattoso L. H. C. 2012Application of Polysaccharide Hydrogels in Adsorption and Controlled-Extended Release of Fertilizers Processes. 123 4 2291 2298
Buyanov A. L. Gofman I. V. Revel’skaya L. G. Khripunov A. K. Tkachenko A. A. 2010Anisotropic swelling and mechanical behavior of composite bacterial cellulose-poly(acrylamide or acrylamide-sodium acrylate) hydrogels. 3 1 102 111
Cao X. D. Habibi Y. Magalhaes W. L. E. Rojas O. J. Lucia L. A. 2011Cellulose nanocrystals-based nanocomposites: fruits of a novel biomass research and teaching platform. 100 8 1172 1176
Capadona J. R. Shanmuganathan K. Triftschuh S. Seidel S. Rowan S. J. Weder C. 2009Polymer Nanocomposites with Nanowhiskers Isolated from Microcrystalline Cellulose. 10 4 712 716
Capadona J. R. Shanmuganathan K. Tyler D. J. Rowan S. J. Weder C. 2008Stimuli-responsive polymer nanocomposites inspired by the sea cucumber dermis. 319 5868 1370 1374
Changsarn S. Mendez J. D. Shanmuganathan K. Foster E. J. Weder C. Supaphol P. 2011Biologically Inspired Hierarchical Design of Nanocomposites Based on Poly(ethylene oxide) and Cellulose Nanofibers. 32 17 1367 1372
Chen D. Liu T. X. Zhou X. P. Tjiu W. C. Hou H. Q. 2009Electrospinning Fabrication of High Strength and Toughness Polyimide Nanofiber Membranes Containing Multiwalled Carbon Nanotubes. 113 29 9741 9748
Dong H. Strawhecker K. E. Snyder J. F. Orlicki J. A. Reiner R. S. Rudie A. W. 2012Cellulose nanocrystals as a reinforcing material for electrospun poly(methyl methacrylate) fibers: Formation, properties and nanomechanical characterization. 87 4 2488 2495
Duran N. Lemes A. P. Duran M. Freer J. Baeza J. 2011A Minireview of Cellulose Nanocrystals and Its Potential Integration as Co-Product in Bioethanol Production. 56 2 672 677
Eichhorn S. J. 2011Cellulose nanowhiskers: promising materials for advanced applications. 7 2 303 315
Filson P. B. Dawson-Andoh B. E. Schwegler-Berry D. 2009Enzymatic-mediated production of cellulose nanocrystals from recycled pulp. 11 11 1808 1814
Gomez-Tejedor J. A. Van Overberghe N. Rico P. Ribelles J. L. G. 2011Assessment of the parameters influencing the fiber characteristics of electrospun poly(ethyl methacrylate) membranes. 47 2 119 129
Greiner A. Wendorff J. H. 2007Electrospinning: A fascinating method for the preparation of ultrathin fibres. 46 30 5670 5703
Habibi Y. Heim T. Douillard R. 2008AC electric field-assisted assembly and alignment of cellulose nanocrystals. 46 14 1430 1436
Habibi Y. Lucia L. A. Rojas O. J. 2010Cellulose Nanocrystals: Chemistry, Self-Assembly, and Applications. 110 6 3479 3500
Herrera Vargas. N. 2010Aligned cellulose nanofibers prepared by electrospinning. (Vol. Master, 58Luleå: Luleå University of Technology.
Hou H. Q. Ge J. J. Zeng J. Li Q. Reneker D. H. Greiner A. Cheng S. Z. D. 2005Electrospun polyacrylonitrile nanofibers containing a high concentration of well-aligned multiwall carbon nanotubes. 17 5 967 973
Huang J. Liu L. Yao J. M. 2011Electrospinning of Bombyx mori Silk Fibroin Nanofiber Mats Reinforced by Cellulose Nanowhiskers. 12 8 1002 1006
Khalil H. P. S. A. Bhat A. H. Yusra A. F. I. 2012Green composites from sustainable cellulose nanofibrils: A review. 87 2 963 979
Kim J. T. Netravali A. N. 2010Mechanical, Thermal, and Interfacial Properties of Green Composites with Ramie Fiber and Soy Resins. 58 9 5400 5407
Kvien I. Tanem B. S. Oksman K. 2005Characterization of cellulose whiskers and their nanocomposites by atomic force and electron microscopy. 6 6 3160 3165
Li Y. 2010Emulsion electrospinning of nanocrystalline cellulose reinforced nanocomposite fibres. (Vol. Master of Applied Science, 115Vancouver: University of British Columbia.
Liang S. M. Zhang L. N. Li Y. F. Xu J. 2007Fabrication and properties of cellulose hydrated membrane with unique structure. 208 6 594 602
Lu P. Hsieh Y. L. 2009Cellulose nanocrystal-filled poly(acrylic acid) nanocomposite fibrous membranes. 20 41 415604
Lu X. F. Wang C. Wei Y. 2009One-Dimensional Composite Nanomaterials: Synthesis by Electrospinning and Their Applications. 5 21 2349 2370
Magalhaes W. L. E. Cao X. D. Lucia L. A. 2009Cellulose Nanocrystals/Cellulose Core-in-Shell Nanocomposite Assemblies. 25 22 13250 13257
Mangalam A. P. Simonsen J. Benight A. S. 2009Cellulose/DNA Hybrid Nanomaterials. 10 3 497 504
Martinez-Sanz M. Olsson R. T. Lopez-Rubio A. Lagaron J. M. 2011Development of electrospun EVOH fibres reinforced with bacterial cellulose nanowhiskers. Part I: Characterization and method optimization. 18 2 335 347
Medeiros E. S. Mattoso L. H. C. Ito E. N. Gregorski K. S. Robertson G. H. Offeman R. D. Wood D. F. Orts W. J. Imam S. H. 2008Electrospun Nanofibers of Poly(vinyl alcohol) Reinforced with Cellulose Nanofibrils. 2 3 231 242
Moon R. J. Martini A. Nairn J. Simonsen J. Youngblood J. 2011Cellulose nanomaterials review: structure, properties and nanocomposites. 40 7 3941 3994
Nakayama A. Kakugo A. Gong J. P. Osada Y. Takai M. Erata T. Kawano S. 2004High mechanical strength double-network hydrogel with bacterial cellulose. 14 11 1124 1128
Oksman K. Mathew A. P. Bondeson D. Kvien I. 2006Manufacturing process of cellulose whiskers/polylactic acid nanocomposites. 66 15 2776 2784
Olsson R. T. Kraemer R. Lopez-Rubio A. Torres-Giner S. Ocio M. J. Lagaron J. M. 2010Extraction of Microfibrils from Bacterial Cellulose Networks for Electrospinning of Anisotropic Biohybrid Fiber Yarns. 43 9 4201 4209
Sullivan O. A. C. 1997Cellulose: the structure slowly unravels. 4 3 173 207
Park W. I. Kang M. Kim H. S. Jin H. J. 2007Electrospinning of Poly(ethylene oxide) with Bacterial Cellulose Whiskers. 249-250 1 289 294
Peng B. L. Dhar N. Liu H. L. Tam K. C. 2011Chemistry and Applications of Nanocrystalline Cellulose and Its Derivatives: A Nanotechnology Perspective. 89 5 1191 1206
Peresin M. S. Habibi Y. Vesterinen A. H. Rojas O. J. Pawlak J. J. Seppala J. V. 2010aEffect of Moisture on Electrospun Nanofiber Composites of Poly(vinyl alcohol) and Cellulose Nanocrystals. 11 9 2471 2477
Peresin M. S. Habibi Y. Zoppe J. O. Pawlak J. J. Rojas O. J. 2010bNanofiber Composites of Polyvinyl Alcohol and Cellulose Nanocrystals: Manufacture and Characterization. 11 3 674 681
Ramirez M. A. 2010Cellulose Nanocrystals Reinforced Electrospun Poly(lactic acid) Fibers as Potential Scaffold for Bone Tissue Engineering. (Vol. Master of Science, 75Raleigh: North Carolina State University.
Reneker D. H. Yarin A. L. 2008Electrospinning jets and polymer nanofibers. 49 10 2387 2425
Rojas O. J. Montero G. A. Habibi Y. 2009Electrospun Nanocomposites from Polystyrene Loaded with Cellulose Nanowhiskers. 113 2 927 935
Rusli R. Eichhorn S. J. 2008Determination of the stiffness of cellulose nanowhiskers and the fiber-matrix interface in a nanocomposite using Raman spectroscopy. 93 3pp.
Samantha A. Meenach K. W. A. Zach J. Hilt 2009. New York: Springer.
Samir M. A. S. A. Alloin F. Dufresne A. 2005Review of recent research into cellulosic whiskers, their properties and their application in nanocomposite field. 6 2 612 626
Saravanan P. Raju M. P. Alam S. 2007A study on synthesis and properties of Ag nanoparticles immobilized polyacrylamide hydrogel composites. 103 2-3 278 282
Schexnailder P. Schmidt G. 2009Nanocomposite polymer hydrogels. 287 1 1 11
Shanmuganathan K. Capadona J. R. Rowan S. J. Weder C. 2010Bio-inspired mechanically-adaptive nanocomposites derived from cotton cellulose whiskers. 20 1 180 186
Siro I. Plackett D. 2010Microfibrillated cellulose and new nanocomposite materials: a review. 17 3 459 494
Spagnol C. Rodrigues F. H. A. Neto A. G. V. C. Pereira A. G. B. Fajardo A. R. Radovanovic E. Rubira A. F. Muniz E. C. 2012aNanocomposites based on poly(acrylamide-co-acrylate) and cellulose nanowhiskers. 48 3 454 463
Spagnol C. Rodrigues F. H. A. Pereira A. G. B. Fajardo A. R. Rubira A. F. Muniz E. C. 2012bSuperabsorbent hydrogel composite made of cellulose nanofibrils and chitosan-graft-poly(acrylic acid). 87 3 2038 2045
Sturcova A. Davies G. R. Eichhorn S. J. 2005Elastic modulus and stress-transfer properties of tunicate cellulose whiskers. 6 2 1055 1061
Tashiro K. Kobayashi M. 1991Theoretical Evaluation of Three-Dimensional Elastic-Constants of Native and Regenerated Celluloses: Role of Hydrogen-Bonds. 32 8 1516 1530
Vandamme E. J. De Baets S. Vanbaelen A. Joris K. De Wulf P. 1998Improved production of bacterial cellulose and its application potential. 59 1-3 93 99
Wang B. Cai Q. Zhang S. Yang X. P. Deng X. L. 2011The effect of poly (L-lactic acid) nanofiber orientation on osteogenic responses of human osteoblast-like MG63 cells. 4 4 600 609
Wu Y. T. Zhou Z. Fan Q. Q. Chen L. Zhu M. F. 2009Facile in-situ fabrication of novel organic nanoparticle hydrogels with excellent mechanical properties. 19 39 7340 7346
Xiang C. H. Joo Y. L. Frey M. W. 2009Nanocomposite Fibers Electrospun from Poly(lactic acid)/Cellulose Nanocrystals. 3 2 147 155
Zhang Y. Yu J. R. Zhou C. J. Chen L. Hu Z. M. 2010Preparation, Morphology, and Adhesive and Mechanical Properties of Ultrahigh-Molecular-Weight Polyethylene/SiO2 Nanocomposite Fibers. 31 4 684 690
Zhou C. J. Qiu X. Y. Zhuang Q. X. Han Z. W. Wu Q. L. 2012aIn situ polymerization and photophysical properties of poly(p-phenylene benzobisoxazole) /multiwalled carbon nanotubes composites. 124 6 4740 4746
Zhou C. J. Chu R. Wu R. Wu Q. L. 2011aElectrospun Polyethylene Oxide/Cellulose Nanocrystal Composite Nanofibrous Mats with Homogeneous and Heterogeneous Microstructures. 12 7 2617 2625
Zhou C. J. Wang Q. W. Wu Q. L. 2012bUV-initiated crosslinking of electrospun poly(ethylene oxide) nanofibers with pentaerythritol triacrylate: Effect of irradiation time and incorporated cellulose nanocrystals. 87 2 1779 1786
Zhou C. J. Wang S. F. Zhang Y. Zhuang Q. X. Han Z. W. 2008aIn situ preparation and continuous fiber spinning of poly(p-phenylene benzobisoxazole) composites with oligo-hydroxyamide-functionalized multi-walled carbon nanotubes. 49 10 2520 2530
Zhou C. J. Wang S. F. Zhuang Q. X. Han Z. W. 2008bEnhanced conductivity in polybenzoxazoles doped with carboxylated multi-walled carbon nanotubes. 46 9 1232 1240
Zhou C. J. Wu Q. L. 2011A novel polyacrylamide nanocomposite hydrogel reinforced with natural chitosan nanofibers. 84 1 155 162
Zhou C. J. Wu Q. L. Yue Y. Y. Zhang Q. G. 2011bApplication of rod-shaped cellulose nanocrystals in polyacrylamide hydrogels. 353 1 116 123
Zhou C. J. Wu Q. L. Zhang Q. G. 2011cDynamic rheology studies of in situ polymerization process of polyacrylamide-cellulose nanocrystal composite hydrogels. 289 3 247 255
Zhou C. J. Yang W. M. Yu Z. N. Zhou W. L. Xia Y. M. Han Z. W. Wu Q. L. 2011dSynthesis and solution properties of novel comb-shaped acrylamide copolymers. 66 3 407 417
Zhou C. J. Zhuang Q. X. Qian J. Li X. X. Han Z. W. 2008cA simple modification method of multiwalled carbon nanotube with polyhydroxyamide. 37 3 254 255
Zoppe J. O. Peresin M. S. Habibi Y. Venditti R. A. Rojas O. J. 2009Reinforcing Poly(epsilon-caprolactone) Nanofibers with Cellulose Nanocrystals. 1 9 1996 2004